This is an open access article published under an ACS AuthorChoice License, which permits copying and redistribution of the article or any adaptations for non-commercial purposes.
Hybrid Multilayered Plasmonic Nanostars for Coherent Random Lasing Battulga Munkhbat,† Johannes Ziegler,† Hannes Pöhl,† Christian Wörister,† Dmitry Sivun,† Markus C. Scharber,‡ Thomas A. Klar,† and Calin Hrelescu*,† †
Institute of Applied Physics, and ‡Linz Institute for Organic Solar Cells/Institute of Physical Chemistry, Johannes Kepler University Linz, 4040 Linz, Austria S Supporting Information *
ABSTRACT: Here, we report that hybrid multilayered plasmonic nanostars can be universally used as feedback agents for coherent random lasing in polar or nonpolar solutions containing gain material. We show that silver-enhancement of gold nanostars reduces the pumping threshold for coherent random lasing substantially for both a typical dye (R6G) and a typical ﬂuorescent polymer (MEH-PPV). Further, we reveal that the lasing intensity and pumping threshold of random lasers based on silver-enhanced gold nanostars are not inﬂuenced by the silica coating, in contrast to gold nanostar-based random lasers, where silica-coated gold nanostars support only ampliﬁed spontaneous emission but no coherent random lasing.
1. INTRODUCTION Triggered by initial reports on lasers with mirrorless feedback,1,2 random lasers with noncoherent (which essentially is ampliﬁed spontaneous emission, ASE)1−4 and coherent feedback5−7 moved closer in the focus of extensive research activities.8,9 Coherent light ampliﬁcation using high refractive index dielectric or metallic nanostructures inside a gain medium can be seen as a promising alternative to conventional lasers. While a conventional laser requires accurate fabrication and extremely precise alignment of the resonator, the resonator in a coherent random laser is realized by randomly distributed scattering nanoparticles forming closed-loops for photons.10−12 This permits a cheap and easy fabrication method, making coherent random lasers an attractive alternative to conventional lasers in a manifold of potential applications, ranging from smart sensors and medical diagnostics,13−16 to lighting devices9 and displays.17 Noble metal nanoparticles exhibiting localized plasmon resonances18 provide two beneﬁcial features for coherent random lasers: much higher scattering cross sections than dielectric nanoparticles19,20 and high ﬁeld enhancements close to their surface, associated with localized plasmons.18,21 It turns out that star-shaped gold nanoparticles, so-called gold nanostars, outperform conventionally shaped gold nanoparticles such as spheres and rods in terms of coherent random lasing.22 Gold nanostars exhibit multiple plasmon resonances in the red and near-infrared spectral region.23−26 These plasmon resonances associated with the tips of the gold nanostars lead to large and spectrally broad-band scattering cross sections as well as extremely strong ﬁeld enhancements localized at the tips,23−26 key features for coherent random lasers. © 2016 American Chemical Society
However, despite all of the eﬀorts on plasmon-mediated coherent random lasing,27−33 there are no reports on hybrid multilayered plasmonic nanostars-based coherent random lasing. Here, we report on the development of hybrid multilayered plasmonic nanostars, which can be mixed with gain materials dissolved in either polar or nonpolar solvents. Two diﬀerent, but in terms of optical properties similar, gain materials, a dye molecule and a light-emitting polymer, were dispersed in polar or nonpolar solvents, respectively. For extremely low pumping thresholds, the solutions containing gain material and silverenhanced and silica-coated nanostars exhibit spectrally narrow lasing modes, typical for coherent random lasing. Further, we show that silver-enhancement of the gold nanostars reduces the pumping threshold for nanostar-based random lasing. Additionally, we reveal that the silica coating nearly does not inﬂuence the operation of the silver-enhanced gold nanostarbased random lasers in terms of lasing intensity and pumping threshold, in contrast to gold nanostar-based random lasers, where only ASE and no coherent random lasing was observed for the silica-coated gold nanostars.
2. EXPERIMENTAL SECTION 2.1. Materials. Silver nitrate (AgNO3, 99.9999%), gold(III) chloride trihydrate (HAuCl4·3H2O), L-ascorbic acid (AA), tetraethyl orthosilicate (TEOS), trisodium citrate dihydrate, 1 Received: June 7, 2016 Revised: October 1, 2016 Published: October 4, 2016 23707
DOI: 10.1021/acs.jpcc.6b05737 J. Phys. Chem. C 2016, 120, 23707−23715
The Journal of Physical Chemistry C
Figure 1. (a) Sketch of the synthesis route for hybrid multilayered nanostars. SEM images of a representative (b) AuNSt and of representative (c) AuAgNSts. TEM images of a representative (d) [email protected]
and (e) [email protected]
The scale bars are 100 nm. Insets: Schematics of the corresponding nanostars illustrating the layered composition.
chloride (HAuCl4), hereafter called growth solution. The pH was adjusted by adding 10 μL of 1 N hydrochloric acid (HCl). Subsequently, 100 μL of 2 mM silver nitrate (AgNO3) and 50 μL of 0.1 M ascorbic acid (AA) were simultaneously added to the growth solution under vigorous stirring. The nanostars were functionalized with hexadecyltrimethylammonium bromide (CTAB); that is, 100 μL of 0.1 M CTAB was added to the growth solution, which was left stirring for 5 min. The solutions containing AuNSts were washed by centrifugation (2000 rcf for 20 min), and redispersed in a 10 mL of 1 mM aqueous CTAB solution. Figure 1a shows the SEM image of a representative AuNSt. The scale bar is 100 nm. More exemplary SEM images are shown in Figure S1. Such AuNSts with long and sharp tips, pointing in arbitrary directions, exhibit multiple plasmon resonances, strong ﬁeld enhancements located at their tips, as well as large scattering cross sections.26 2.2.2. Synthesis of Silver-Enhanced Gold Nanostars. For the silver-enhanced gold nanostars (AuAgNSts), we followed a method that was inspired by the method reported by Fales et al.36 5 μL of 0.1 M AgNO3 and an equivalent volume of 0.1 M AA were added as a precursor and as a reducing agent, respectively, under vigorous stirring to 1 mL of CTABfunctionalized AuNSts in solution. After 15 min, the silver enhanced gold nanostars were puriﬁed by centrifugation at 2000 rcf for 10 min, discarding the supernatant, and redispersed in 1 mL of distilled water. Figure 1b shows an SEM image of representative AuAgNSts. The AuAgNSts still exhibit sharp tips, but the branch length of the previously long gold nanostar tips protruding from the core of the nanostars is reduced while the core diameter is increased due to the silver-enhancement. Several examples of SEM images can be found in Figure S2. The exact silver shell thickness of the AuAgNSts can hardly be measured precisely with a TEM, due to the limited material contrast. However, we can distinguish between the gold nanostar and the silver shell in high angle annular dark ﬁeld TEM images, so that we estimate the silver shell thickness to be in the range of 20 nm around the core of the gold nanostar (an example is shown in Figure S3). Further, from elemental line and mapping analysis of representative AuAgNSts using energy dispersive X-ray spectroscopy (EDX), we assume that the apexes of the tips are also covered by a very thin (